A Study of Hydrogen Effects on Fracture Behavior of Radioactive Waste Storage Tanks Final Report To United States Department of Energy Office of Energy Research Washington DC 20585 Contract: DE-FG05-92ER 75784 (10/92 - 9/94) G te * v c Gte* by K. Linga Murty (Co-PI) Thomas S. Elleman (Co-PI - 10/92-11/93) Department of Nuclear Engineering North Carolina State University Raleigh, NC mum A L s DiSTRiBUTO 0F-7HB NCSU IS ONL1»ID STER
A Study of Hydrogen Effects on Fracture Behaviorof
Radioactive Waste Storage Tanks
United States Department of EnergyOffice of Energy ResearchWashington DC 20585
Contract: DE-FG05-92ER 75784(10/92 - 9/94)
G te *v cG te *
byK. Linga Murty (Co-PI)
Thomas S. Elleman (Co-PI - 10/92-11/93)
Department of Nuclear EngineeringNorth Carolina State University
IS ONL1»ID STER
This report was prepared as an account of work sponsored by an agency of theUnited States Government Neither the United States Government nor any agencythereof, nor any of their employees, makes any warranty, express or implied, orassumes any legal liability or responsibility for the accuracy, completeness, or use-fulness of any information, apparatus, product, or process disclosed, or represenuthat its use would not infringe privately owned rights. Reference herein to any spe-cific commercial product, process, or service by trade name, trademark, manufac-turer, or otherwise does not necessarily constitute or imply its endorsement, recom-mendation, or favoring by the United States Government or any agency thereof.The views and opinions of authors expressed herein do not necessarily state orreflect those of the United States Government or any agency thereof.
Portions of this document may be illegiblein electronic image products. Images areproduced from the best available originaldocument.
A Study of Hydrogen Effects on Fracture Behaviorof
^Radioactive Waste Storage Tanks
The processing of high-level radioactive wastes now stored at Hanford andSavannah River Laboratories will continue over many years and it will be necessaryfor some of the liquids to remain in the tanks until well into the next century.Continued tank integrity is therefore an issue of prime importance and it will benecessary to understand any processes which could lead to tank failure. Hydrogenembrittlement resulting from absorption of radiolytic hydrogen could alter tankfracture behavior and be an issue in evaluating the effect of stresses on the tanksfrom rapid chemical oxidation-reduction reactions. The intense radiation fields insome of the tanks could be a factor in increasing the hydrogen permeation ratesthrough protective oxide films on the alloy surface and be an additional factor incontributing to embrittlement.
The project was initiated in October 1992 for a two year period to evaluatehydrogen uptake in low carbon steels that are representative of storage tanks. Steelspecimens were exposed to high gamma radiation fields to generate radiolytichydrogen and to potentially alter the protective surface films to increase hydrogenuptake. Direct measurements of hydrogen uptake were made using tritium as atracer and fracture studies were undertaken to determine any alloy embrittlement.The rates of hydrogen uptake were noted to be extremely low in the experimentalsteels. Gamma radiation did not reveal any significant changes in the mechanicaland fracture characteristics following exposures as long as a month. It is highlydesirable to investigate further the tritium diffusion under stress in a cracked bodywhere stress-assisted diffusion is expected to enhance these rates. More importantly,since welds are the weakest locations in the steel structures/ the mechanical andfracture tests should be performed on welds exposed to tritium with and withoutstressed crack-fronts.
DoE Final Report / 1995 page 2
The project supported three graduate students : Ms. Nevenka Bierny
(Materials Science & Engineering), Mr. Stephen Kass (Nuclear Engineering) and Mr.
Patrick Markle (Materials Science & Engineering). Mr. Kass completed his Master of
Nuclear Engineering (MNE) degree in Dec. 1994 while Mr. Markle completed his
Master of Science (MS) degree in June 1995. The above two students did their
project/thesis work on different but related topics : Mr. Kass (12/94) - Radiation
Embrittlement and Dynamic Strain Aging in Mild Steels and Armco Iron, and Mr.
Markle (3/95) -Creep and Creep Crack Growth In A508B Pressure Vessel Steel.
DoE Final Report / 1995 page 3
Large carbon-steel tanks at the Savannah River Laboratory in Aiken, South
Carolina and the Hanford facility in Richland, Washington are the principal storage
containers for the chemical processing solutions that were used in the preparation
of weapons grade plutonium. Additional radioactive waste solutions are stored in
stainless steel tanks at Idaho Falls, Idaho and in carbon-steel tanks at the West
Valley reprocessing facility in New York. Reprocessing operations at these locations
have generated solutions of radioactive waste for over forty years and have
remained in these waste storage tanks. Initially, the storage tanks were unannealed,
single wall carbon steel (A285-B) tanks without any special weld materials; later,
additional tanks were constructed with stress relieved, carbon steel (A516-70) double
walls. Illustrations of the single and double shelled tanks are included in figures 1.1
(a) and 1.1 (b) respectively. The chemical compositions of the materials used for the
single and double walled tanks are shown below in Table 1.1.
Chemical Compositions (wt %) of Waste Tank Steels
The compositions of the original solutions in the tanks were known, butsubsequent transfers of solutions have made the compositional records of severaltanks ambiguous. The tank solutions have complex compositions, and includeinorganic nitrates, nitrites, traces of halides, ferrocyanides, and a variety of inorganicsalts. The pH of the tank solutions is maintained at approximately 10, and nitritesare added to mitigate the effects of stress corrosion cracking. Only the SavannahRiver Laboratory site maintains a program to control the chemical conditionswithin the tanks.
DoE Final Report / 1995 page 4
Figure 1.1Illustrations of (a) Single (top) and (b) Double (bottom) Shelled Tanks
Liquid Observation Well\ , Camera
Surface Level Profaa \ Observation(FIC or Manual T a p e s ) \ ™ \ Solids L(.v.l po,nt Dams Elevation
Center I / Bench MarkPump Pll Exhauster fill-Meat
2911 IMG 2
Leak . AnnulusDetection P u m p
Surface Level Probe(FIC & Manual Tape)
olids Level Detector /Flow Monitor
Dome Elevation - = / TemperatureBench Mark S /Thermocouple
DoE Final Report / 1995 page 5
Leaks were noted several years ago in the single wall tanks when tank levelsdecreased and radioactive nuclides were detected at sampling stations near the wastetanks. Leaking tanks were pumped dry and the remaining solution was transferredto the newer double wall tanks which have proven to be more structurally sound.Leaks have required 100 of the 149 single wall tanks to be emptied. The single walltank failures were attributed to stress corrosion cracking at the Savannah River andHanford waste sites. Both storage facilities initiated programs to chemically controlthe tank contents in an attempt to reduce the amount of stress corrosion cracking.These programs prescribed elevated nitrite concentrations and pH conditions tolimit the effect of stress corrosion cracking on the surface of the tanks. Although sitepersonnel believe that these measures have reduced the rate of tank failures, theystill consider the single wall tanks to be susceptible to failure in the future.
The double walled tanks were made with greater attention to the selection ofthe materials, and in most cases were annealed in-situ. Their performance has beensatisfactory but the harsh radioactive environment makes the pitting and corrosionprocess difficult to monitor. A summary of the various tanks and their locations areprovided in Table 1.2.
Table 1.2Status of Waste Storage Tanks
Total Storage Tanks
A failed tank does not imply that an unsafe condition exists at the facility inquestion, since failed tanks are pumped dry to stabilize the radioactive materialwhich exists as a dry sludge in the bottom of the tank. Tank failure does limit thestorage capabilities of the sites and there is presently little unused storage capacity toaccommodate additional solution storage. There has also been concern about
DoE Final Report / 1995 page 6
chemical reactions which may place the integrity of the tanks in jeopardy if thetanks experience an unanticipated load(s). Several tanks are known to generategaseous mixtures of hydrogen and nitrous oxides.
The Hartford and Savannah River sites anticipate the use of a glassifkationoperation for processing radioactive waste. Both sites have glassification plantsplanned or under construction; however, these facilities would be able to processonly one tank per year per site. The emptying and removal of tanks from service is alengthy process that will probably not be fully operational for at least ten years. Tankintegrity will, therefore, need to be assured for a long time.
The purpose of this discussion is to emphasize the significance andimportance of having a solid understanding of the processes and conditions thatwill lead to potential failure(s) of waste storage tanks. While the tanks appear to bepresently stabilized, there is considerable motivation to understand the long termcorrosion and failure processes that could compromise tank integrity in the future.
2. Hydrogen Effects
One of the processes that could produce considerable degradation in thestructural integrity of the waste tank alloys is the buildup of atomic hydrogen atgrain boundaries. Favorable conditions exist for hydrogen adsorption at a crack tip,where the bare metal is not protected by an oxide layer. Rapid diffusion of hydrogento crack fronts has been known to produce severe embrittlement in many differentmaterials. Hydrogen embrittlement of carbon steels is a well known process that hasbeen the subject of numerous studies and investigations. Embrittlement would notgenerally be expected under the chemical conditions in which radioactive wastes arestored, however, the radiation environment presents unusual conditions whichcould alter the normal metallurgical behavior of the alloys.
The intense radiation fields that have been associated with decayingradioactive species continuously generate hydrogen and hydroxyl free radicals thatreact to form gaseous hydrogen and hydrogen peroxide. The combination ofcontinuos production of atomic hydrogen and the exposure of the internal tank walloxide layers could alter the normal permeation behavior of the surface oxide. It ispossible that these oxide layers are altered in such a way that increases the access ofatomic hydrogen to the bulk metal. The research literature has little information pn
DoE Final Report / 1995 — — — . . _ _ — —
the effects of radiation fields in promoting hydrogen adsorption. However, it isgenerally assumed that the destruction of the protective oxide surface layers wouldlead to rapid hydrogen uptake. It is plausible that the unique chemical environmentassociated with stored wastes, in conjunction with the radiation field would alterthe hydrogen uptake rates and the subsequent embrittlement. The research issuesdiscussed here are illustrated in Fig. 2.1.
1. Can Radiation Fields Produce Accelerated HydrogenUptake?
A. Free Radical Formation:Hydrogen Permeation
In Radiation Fields
H2 => H- + H-H2O =*> H- + OH-H- + H- =*> H2
•OH + O H =>H2O2
B. Breakdown of Oxide Protective Films
2, If Accelerated Hydrogen Uptake Occurs,Will Substrate Fracture Behavior be Degraded?
Figure 2.1Issues Related to Hydrogen Effects
DoE Final Report I 1995 page 8
In this study, samples of steels commonly used in waste tanks were placed in
aqueous solutions which contained a known amount of tritium and were
subsequently exposed to a gamma ray field of approximately 40,000 rads/hr. This
dose rate is approximately ten times those encountered in the waste tanks. The
hydrogen adsorption and the consequent mechanical properties of the samples were
examined to determine if the gamma rays had any effect on hydrogen migration and
subsequent fracture properties.
3. Experimental Methods
This section provides a description of the experimental techniques and
procedures that were employed in this research. It includes a description of the
materials that were tested, their chemical compositions, microstructures, and tensile
properties of unirradiated specimens. Details are provided on the technique used to
irradiate the specimens, procedures used to determine the amount of tritium
diffusion and its effect on mechanical properties of the steel. Methods and
procedures for sample fabrication, performance of the tensile tests and data
recording are also included.
3.1.1 Chemical Composition
Three different steels were considered in this research: A516gr70, AISI 1020,
and A354 steel. Their chemical compositions are included in Table 3.1. The 1020
steel was acquired from Duke Power Company (courtesy Mr. Ray McCoy) while the
A516gr70 and A354 steels were procured from HUB Incorporated.
3.1.2 Optical Metallography
Microstructures of unirradiated A516 steel, AISI 1020 steel, and A354 steel are
shown in figures 3.1 (a), 3.1 (b) and 3.1 (c). All of these materials are categorized as
hypoeutectoid steels, meaning their carbon contents are less than 0.77 weight
percent. The light grains in each micrograph are the primary alpha iron phase
(ferrite) and the dark areas are pearlite. Pearlite is a microconstituent in steel which
has a lamellar structure of alternating layers of ferrite and cementite (Fe3Q.
Average grain sizes for these four steels range between 20 and 40/^m.
DoE Final Report / 1995 page 9
Chemical Composition (wt %) of Experimental Steels
Optical Micrographs of A516 (a), 1020 (b) and A354 (c) Steels
AsnAIS! 1020 A 354
DoE Final Report / 1995 page 10
3.1.3 Mechanical Properties of Unirradiated Iron and Steel
Mechanical characteristics of the unexposed steels were evaluated forsubsequent comparison with the samples exposed to hydrogen and radiation.Tensile tests were performed on a closed loop Instron servohydraulic tensile testingmachine (as described later) at ambient temperature and at a strain rate of lxlCK s'1.The mechanical properties of these archive materials are summarized below inTable 3.2.
Mechanical Properties of Unirradiated Steel Specimens
0.2% OffsetYield Stress
3.2 Radiation Arrangement
3.2.1 Sample Irradiation
A capped aluminum container (2" diameter and 3" high), was fabricated tohold the Charpy (three-point bend) and tensile specimens while in the gamma cell.The photographs of the container are included in figure 3.2 while a schematic of thecontainer is shown in figure 3.3.
DoE Final Report / 1995 page 11
Figure 3.2Photographs of Aluminum Container for Gamma Irradiation
DoE Final Report / 1995 page 12
Figure 3.3 'Schematic of the Aluminum Container for Gamma Irradiation
Relief Valve Fitting for electricalconnections
A fitting was machined into the cap of the aluminum container toaccommodate a thermocouple which was used to control and monitor thetemperature during irradiation. A relief valve was also placed on the cap of thecontainer (at the center) to vent any pressure that may have built up during hightemperature exposures. Three-point bend and tensile specimens were placed in thealuminum container with a 20 ml solution that included a tritium tracer.Specimens were sealed in the container and irradiated in a Co-60 gamma cell atroom temperature, 80°C and 100°C.
A Gamacell model 220, manufactured by Atomic Energy of Canada Ltd., wasused for all sample exposures. Gamma dose rates were determined using thefollowing decay rate provided by the manufacturer:
DoE Final Report / 1995 page 13
where, d is the gamma dose in rads/hr, /„ is May 29,1970 and t is the date of use. All
gamma irradiations performed in this study were on the order of 45000 rads/hr.
The Gammacell 220 is a Cobalt-60 irradiation chamber that is designed foruse in an unshielded room. The unit consists of an annular source permanentlyenclosed within a lead shield, a cylindrical drawer and a drive mechanism to movethe drawer up or down along the center line of the source. The drawer has achamber to carry samples to be irradiated from outside the shield to the source.Samples approximately six inches in diameter and eight inches in height can beaccommodated in the chamber. Electrical and mechanical connections can beintroduced into the sample chamber through an access tube in the upper portion ofthe drawer. A photograph and diagram of the gamma cell are included in figures 3.4and 3.5 respectively.
High temperature gamma radiation exposures were made to enhancehydrogen diffusion into the steel which may result in changes in the mechanicalproperties of these materials. Standard heating tape was wrapped around thecircumference of the aluminum canister and was connected to a 120V variablepower supply through a thermocouple and a Barber Coleman temperaturecontroller. The desired temperature was set on the temperature controller whichopened and closed the circuit to the power supply (and the heating tape) dependingon how far the thermocouple temperature was from the desired set point. Tensilesamples were irradiated in distilled water to 80°C and in silicone oil to 100°C.Silicone oil was used for the high temperature irradiations to minirnize thepressure build up in the aluminum container during prolonged exposure times.
DoE Final Report / 1995 page 14
Photograph of the Gamma CellTOP PLUGINTERLOCKMiCROSWITCH
DoE Final Report / 1995 page 15
Detailed Diagram of the GAMACELL 220
ne s»euj HUGOffAWCM TO*
u n r r wrenuooi WCJ»SVHTCW«
cokt^M ooo* >UNOI.C a LATCH
90UKS KMCK. JUMMSLy (ttt OCtM.1
C M « U SOT TOM
OHMClt MMUM. CtM«
TDK MCOU KLtCTlW WITCH
GAMACELL 220GENERAL DIMENSIONS
DoE Final Report / 1995 page 16
3.3 Sample Preparation and Testing
Tensile specimens were fabricated from the three different grades of steel usedfor this study: A516gr70, AISI 1020, and A354. Three point bend specimens weremade from A516gr70 only. The three point bend samples were used to measure thediffusion coefficient of hydrogen in the steel. To accomplish this, the specimenswere exposed in gamma cell while immersed in a solution that contained tritium.After gamma ray exposure, layers of the steel sample were removed viaelectropolishing. The electropolish solution was then counted in a liquid scintillatorcounter to measure the tritium activity as a function of polish depth. Tensilespecimens were fabricated to determine the effect of gamma rays on mechanicalproperties at room and elevated temperatures. Samples were immersed in distilledwater (without a tritium tracer) and silicone oil (for high temperature irradiations),irradiated and then examined for changes in the mechanical properties such asductility, yield strength, and ultimate tensile strength. An apparatus was alsodesigned and constructed to irradiate three point bend samples under loadedconditions. A photograph of this apparatus is shown in figure 3.6. The original ideawas to examine the effect of stress concentration at the crack front in enhancing themigration of hydrogen (stress-induced diffusion) into the material and subsequentembrittlement of the steel.
Figure 3.6Photograph of Jig for Gamma Irradiation under Load
DoE Final Report / 1995 page 17
4.3.1 Sample Preparation
Three point bend specimens were machined from a block of A516gr70 steel inaccordance with the diagram shown in figure 3.7. A hole was tapped into the top ofthe sample to accommodate a screw, which was attached to the positive lead of apower supply for electropolishing. These specimens were placed into the aluminumcontainer with 2 ml of tritiated water. The tritiated solution was prepared from astock solution of 1-4 Dioxene with an activity of 1.5x10^ dpm/ml. The activity of thetritium solution placed in contact with the steel samples and exposed in the gammacell varied from 0.5 to 50 fiCi/ml. A A516 steel sample was placed in the aluminumcanister with the notch facing down into the tritiated water, ensuring that only oneface was exposed to the tritium. The aluminum container, with the steel sample andtritiated water, was placed in the gamma cell and was exposed for times rangingfrom five days (4.8 Mrad) to 25 days (24 Mrad). The three point bend specimens wereused to determine the diffusion coefficient of hydrogen in the steel.
Figure 3.7Three-Point Bend Specimens
Tensile specimens were fabricated from blocks of A516, AISI 1020, and A354steels in accordance with the diagram provided in figure 3.8. These specimens wereplaced into the aluminum container with 20 ml of distilled water for roomtemperature and 80°C irradiations. High temperature irradiations (100°C) usedsilicone oil in place of water to reduce the amount of liquid lost from evaporation.
DoE Final Report / 1995 page 18
The tensile specimens were used to determine the mechanical property changes inthe steel samples following gamma ray exposures. Tritium tracers were not placedin the water or oil solutions since these samples were not used to determinehydrogen diffusion gradients or concentrations into the steel.
Figure 3.8Drawing of Tensile Specimens
3.3.2 Sample Testing
188.8.131.52 Tritium Tracer Measurement
A516 steel samples were placed in a tritiated solution and were irradiated inthe Gammacell 220 to a specific gamma ray dose. The three point bend samples wereremoved from the aluminum container after irradiation and were prepared forelectropolishing and liquid scintillation counting to determine the concentration oftritium in the steel, as a function of depth, after exposure to gamma rays. Thedimensions of each irradiated steel sample were measured with a micrometer,attached to a 2/56" x 1.25" screw, using gloves and tweezers, and placed into an
DoE Final Report / 1995 page 19
electrolytic solution with a piece of stainless steel (also attached to a 2/56" x 1.25"screw). This arrangement is illustrated in figure 3.9.
Figure 3.9Electro-Polishing Apparatus for Surface Removal
Hewlett PackardGG52A Power Supply
1 hree rantBend Specimen:(Anode)
4V and 0.694 A appliedfrom power supply
2/56" x 1.25" screw
Polish Solution:45% Sulfuric Acid45% Phosphoric Acid10% Water
Proper combinations of current, voltage and polish solution were determinedafter many weeks of experimentation. The sulfuric/phosphoric acid electrolyte, 0.694A and 4V provided conditions for a constant and even polishing rate across the faceof the three point bend specimen. This polishing rate was determined to be 115microns/min. After each polish, 2 ml of the polish solution were removed andplaced into a 20 ml liquid scintillation counting vial. The steel specimen wasremoved from the solution, cleaned and measured with a micrometer to determinethe amount of material removed from the surface. A new electrolyte solution wasprepared and the steel specimen was placed back into the solution for additionalpolishing. Five to six polishes were performed on each steel sample to produce ahydrogen concentration profile of the specimen. A liquid scintillation cocktail wasprepared for each vial which contained 2 ml of the polish solution and 18 ml of theliquid scintillator, Scintiverse II. These vials were counted in Packard 4430 Liquid
DoE Final Report / 1995 page 20
Scintillation Counter along with known standard and background solutions. Thestandard solution was prepared using a 2 ml solution of tritium known to haveI.llxip6 dpm and 18 ml of Scdntiverse II, and the background solution was preparedusing 20 ml of Sciiitiverse II. Three counting windows were programmed into theliquid scintillation counter. Since tritium emits an 18 keV beta particle, the first,second and third windows were set for 0-19 keV, 2-19 keV and 19-1 keV respectively.The vials containing the polish solution, the standard sample, and the backgroundsample were counted three times for an hour each to obtain good counting statistics.The number of counts per minute for each vial was determined by averaging thethree values obtained from the liquid scintillator (since each vial was counted threetimes).
184.108.40.206 Tensile and Three-Point Bend Testing
Tensile specimens of A516, AISI1020, and A354 steels were used to determinethe effect of gamma radiation on the mechanical properties of the steel specimens.Tensile specimens were fabricated in the NCSU Nuclear Engineering Machine Shopfrom forged plates of each particular material. The samples were 1.55 inches longwith a 0.5 inch gage section. Grips were fabricated from tool steel and were used tohold the samples while performing the uniaxial tensile tests. The grips were 35 mmlong and 16 mm wide with a notch and hole to accept the connecting rods and pinsrespectively. A detailed diagram of the grips is included in figure 3.10. Tensile testswere performed on an Instron model 1350 servo-hydraulic testing machine with a1010-AF load cell. A mounting frame was used to prevent from bending the tensilespecimens while being placed in the Instron machine. The upper connecting rodwas attached to the load cell and the lower connecting rod was attached to themovable piston on the Instron machine.
Load-elongation curves were obtained from a Hewlett Packard 7004B X-Ychart recorder that read the output voltage for load and displacement from theInstron machine. Three to four measurements were made along each dimensionand averaged. Tensile tests were performed at a constant strain rate of 1x10*4 s-l atambient test temperature.
DoE Final Report /1995 page 21
Figure 3.10Grip Arrangement for Tensile Tests
upper connection rod
hexa-sew hoieof 1.6 mm dia
DoE Final Report /1995 page 22
4. Results and Discussion
4.1. Tritium Diffusion
Two__.-.solutiOT^^ere:,-ey^uatedj,for.,,,the. electropolishing of carbon steelspecimens. A glycerine-nitric acid based solution exhibited low polish rates andsubstantial pitting of the specimens. A solution consisting of 50% phosphoric acid,50% sulfuric acid produced polishing rates of several mils per hour and a smootherspecimen finish. This solution was selected for the polishing experiments. Aliquotsof tritium tagged solution were added to the polish solution and counted in a liquidscintillation counter using a Scintiverse-II cocktail. The phosphoric-sulfuric acidlowered the counting efficiency from approximately 45% (pure water) to 20%(polish solution) but it was possible to liquid scintillation count the tritium bydirectly adding the polish solution to the scintillation cocktail.
As pointed out, in addition to the liquid scintillation counting of thepolished layers, windowless proportional counter with a pulse height discriminatorwindow to screen noise pulses was assembled to count exposed samples directly.The counter was calibrated with a purchased metal hydride tritium source(Amersham Corp.) and a satisfactory counting plateau was obtained. Specimenswere soaked in tritiated water solution, rinsed" lightly, and counted in theproportional counter. The counting rate was low enough to indicate that littletritium absorbed in the oxide film to produce an undesirable counting backgroundfor the tritium uptake studies.
The hydrogen diffusion experiments yielded the activity versus depth whichare related to the diffusion coefficient, D,
A = Ao exp(-x2/4Dt).
Here, A is the counts/min. Thus semi-log plots of the activity versus square of thedepth [log(A) vs x2] should follow straight lines with slopes from which D can beevaluated.
Typical data obtained are shown in Fig. 4.1 to 4.3 for various time periodsexposed to different total doses : sample #2 (27 Mrad), #3 (13 Mrad) and #4 (16 Mrad).There is a lot of scatter in the data, and straight lines are drawn through log vssquare-of-depth. The slopes of these lines yield Dt from which the diffusion
DoE Final Report / 1995 " ~ page 23
coefficient of tritium in A516 was estimated. From Inactivity) vs time, the diffusion
rates were calculated,
D = 9.71±2.03 x 10-8 0^2/hr (or 2.7xlO-H cm2/sec).
These are very small values compared to published data of hydrogen diffusion in
Depth Profile from A516 Sample #2Irradiation Time = 600.1 hrs
^ 10000 -.
0.00e+0 iOOe-S 4.00e-5 6.00&-5 8.00e-5
Depth squared (cm^2)
Figure 4.2Depth Profile A516 Sample #3
Irradiation Time = 288.1 5
y = 1130.3 * 1 OA(-4O79.Ox) RA2 = 0.890
DoE Final Report / 1995 page 24
Unfortunately, limitations in the budget did not permit evaluation of depthprofiles as a function of temperature. Modifications to the gamma-cell are requiredfor high temperature study. However, mechanical properties were evaluatedfollowing y-radiation exposures at higher temperatures with no tritium tag. Thework performed to date, however, does clearly indicate that the experimentalapproach is appropriate for the proposed study. The original plan of investigatingthe hydrogen uptake at crack front in 3-point bend specimens under load could notbe undertaken.
Figure 4.3Depth Profile from A516 Sample #4
Irradiation Time = 366.18 hrs
0.O 100 :
y = 216.55* 10A(-3858.5x) R*
2 = 0.635
4.2. Effect of y-Radiation on Mechanical Properties
Tensile tests were performed at room temperature on various steel samplesfollowing exposure to y-radiation in the gamma cell. No consistent results wereobtained. Changes in the strength and ductility were nominal, and in many casesthey are within the experimental scatter.
4.2.1. A516 Gr 70 Steel
Figures 4.4 to 4.8 show o-e curves for the unirradiated versus those followingexposures at 100 °C to various times or total doses upto 20 Mrad. We did not findany consistent behavior of either the strength or the ductility, both uniform andtotal elongations.
DoE Final Report / 1995 page 25
Figures 4.4 and 4.8
Stress-Strain Curves for A516 Gr 70 Steel - Effect of Exposure to y-Radiation
190 hrs. @ 100-C
286 hrs. @ 100°C
382 hrs. @ 100-C
200 • f.
382 hrs. @ 100°C
~ 480 hrs. @ 100°C
DoE Final Report / 1995 page 26
Figure 4.9 depicts the effect of dose on fracture strain at 100 °C (in silicone oil
bath) and the strains ranged from about 25% for the as-received to about 19% at 15
Mrad while it increased at the highest dose used, namely 20 Mrad. The
corresponding data on yield and tensile strengths are shown in Fig. 4.10; within the
scatter normally noted for these steels, the variations are regarded as negligible.
Similar trends are noted at room temperature also, and Figures 4.11 and 4.12
document these data. Experiments were performed at 80 °C also (Figures 4.13 and
Effect of Dose (at 100 °Q on Room-Temperature Fracture Strain (A516 Steel)
IA516 Steel at 100C
Figure 4.10Effect of Dose (at 100 °C) on Room-Temperature Yield and Tensile Strengths
'. A516 Stee!
r ° U.T.S.4 Yield Stress
. . . . .
DoE Final Report / 1995 page 27
Effect of Dose on Fracture Strain at 25 °C (A516 Steel)
AST 6 Steel at 25 C
Effect of Dose on Yield and Tensile Strengths at 25 °C (A516 Steel)625
500 I h
• Yield Stress
A516 at 25 C
5 10 15
DoE Final Report / 1995 page 28
Effect of Dose (at 80 °C) on Room-Temperature Fracture Strain (A516 Steel)
^ 20 -
I•OT 1 5
- 8 0
I t i , • i , ,
Figure 4.14Effect of Dose (at 80 °Q on Room-Temperature Tensile Strength (A516 Steel)
A516 exposed at 80 C
DoE Final Report / 1995 page 29
4.2.2. A354 Steel-
Tests were performed on A354 steel (Table 3.2) following exposure in the
gamma cell at 100 °C. Again, since no discernible changes were noted following
room temperature exposure with and without tritium tag, we first wanted to
examine the relatively high temperature exposure effects. The intention here was to
eventually develop a system to expose the materials to tritiated solution at higher
temperatures so that higher rates of tritium uptake could take place. Figures 4.15
and 4.16 show the dose effects on ductility and strength, and essentially similar (as
per A516 steel) are observed.
Figure 4.15Effect of Dose (at 100 °Q on Room-Temperature Fracture Strain (A354 Steel)
A354 Steel at 100C
10 15 20 25
Figure 4.16Effect of Dose (at 100 °C) on Room-Temperature Yield and Tensile Strengths
a ^• 880
f A354 Steel at 100C
* Yield Stress
DoE Final Report / 1995 page 30
Tests were performed on 1020 steel (Table 3.2) following exposure in the
gamma cell at 100 °C Again, no discernible changes were noted in the fracture
strains (Figure 4.17). As depicted in Fig. 4.18, both the yield and tensile strengths
increased at the initial exposure following which they both decreased with increased
dose. However, the changes are not significant - with a maximum of 50 MPa.
Effect of Dose (at 100 °C) on Room-Temperature
Mechanical Properties (1020 Steel)25
1020 Steel at 100C
• Yield Stress
1020 Steel at 100C j
B ° B \BJ
Figure 4.18 ]
i . . . i . . . ;
DoE Final Report / 1995 page 31
As noted in section 4.1, no significant uptake of tritium was noted in thetritium-tag experiments. Limited amount of 3-point bend tests performed alsorevealed ho discernible changes in the load-displacement curves. As described in theinterim report, specimens were irradiated in solution to an accumulated dose of3.24xlO6 rads and three point bend tests were performed. The results obtainedappeared to be generally consistent with the results for unirradiated specimens andno modification in fracture strength was obtained. Later, a second series ofspecimens were exposed to an accumulated dose of 2.52xlO7 rads which also did notreveal any differences. Thus, most of the mechanical property evaluations weremade using tensile tests.
Majority of the time was spent on getting chemical experiments performedusing tritiated water exposures. The studies on tritium diffusion under stress ofcracked specimens could not be taken up due to the discontinuity of the NEERproject in 1994; only no-cost extensions helped in getting the students complete theirmaster's degree research. It is highly desirable to investigate further the tritiumdiffusion under stress in a cracked body where stress-assisted diffusion is expected toenhance these rates. More importantly, since welds are the weakest locations in thesteel structures, the mechanical and fracture tests should be performed on weldsexposed to tritium with and without stressed crack-fronts.
Mr. Kass completed his MNE (master of nuclear engineering) project byinvestigating dose rate effects and his project work resulted in a technical paperwhich is included in the Appendix. Very interesting and new results were obtainedby comparing the mechanical properties following exposures to total (fast + thermal)neutron radiation versus only fast (using Cd-wrapped) neutron radiation. Effect ofgrain size on the strength following these exposures revealed non-negligible effectsof low-energy neutrons on radiation hardening of steels. Inclusion of thermalneutrons along with fast resulted in further decrease in the source hardening with aslight increase in the friction hardening which revealed a critical grain size belowwhich exposure to total (fast and thermal) neutron spectrum resulted in a slightreduction in the yield stress compared to the exposure to only fast neutrons. This isthe first time such a grain size effect is reported and this is shown to be consistentwith known radiation effects on friction and source hardening terms along with theobservation that low energy neutrons have a nonnegligible effect on the mechanical
DoE Final Report / 1995 ~~~ ' page 32
properties of steels. In ferritic steels, however, despite their small grain size,
exposure to total neutron spectrum yielded higher strengths than exposure to only
fast neutrons. This behavior is consistent with the fact that the source hardening is
small in these alloys and radiation effect is due 'only "to'friction stress.
1. R. K. Mahidhara, T. S. Elleman and K. L. Murty, Corrosion and Filure Processesin High-level Waste Tanks, N. C. State University, Report (LANL - ContractNo. 9-XQ-Y3122-1), Nov. 20 (1992) pp. 1 - 35.
2. R. K. Mahidhara, T. S. Elleman and K. L. Murty, Corrosion Failure Processes inLow Carbon Steels, N. C. State University, Report (LANL - Contract No. 9-XQ-Y3122-1), Nov. 25, (1992) pp. 1-80.
3. R. K. Mahidhara, T. S. Elleman and K. L. Murty, Failure Predictions-RateModels in Low Carbon Steels, N. C. State University, Report (LANL - ContractNo. 9-XQ-Y3122-1), Dec 15, (1992) pp. 1 - 46.
4. G. L. Borsheim and N. W. Korsch,Summary of Single-Shelled Tank WasteStability, Hartford Internal Report (March 1991)
6. "Hanford Seeks Short- and Long-Term Solutions to its Legacy of Waste,"Physics Today 17-21 (March 1992).
7. Ondrejcin, R. S., Chemical Compositions of Supernates Stored in SRP High- Level Waste Tanks, DP-1347 (1974).
8. Ondrejcin, R. S.,Prevention of Stress Corrosion Cracking in Nuclear WasteStorage Tanks, Corrosion/84 (April 1984).
9. Ondrejcin, R. S., et al.,Control of Stress Corrosion Cracking in Storage TanksContaining Radioactive Waste, Nuclear Technology 44:297 (1979).
10. Maness, R. F., Stress Corrosion Cracking of Mild Steel in Nitrate Solutions, _HW-78168 (1963).
11. Costas, L. P. et al., Stress Corrosion Cracking of Carbon Steel in SimulatedWaste Solutions, DP-1023 (1966).
12. "High-Level Waste Tank Systems Structural Integrity Workshop" Red Lion-Hanford House, Richland Washington Feb. 19-20 (1992).
DoE Final Report / 1995 page 33
13. "High-Level Radioactive Waste Tank Task Force Meeting" February 1991,Albuquerque, NM.
14. P. E. Zapp, Inhibiting Pitting of Carbon Steel Exposed to Dilute RadioactiveWaste Slurries, Corrosion 792, (April 1992)
15. A. Ciszewski et al. "Effect of Nonmetatiic Inclusions on the Formation ofMicrocracks in Hydrogen Charged 1% Cr Steel" Conf. Stress Corrosion Crackingand Hydrogen Embrittlement of Iron Base Alloys Unieux-Firminy France(June 12,1973)
16. C. S. Carter and M. V. Hyatt "Review of Stress Corrosion Cracking in Low AlloySteels with Yield Strengths Below 150KSi" Ibid pp. 524-593.
17. R. B. Diegle and W. K. Boyd "The Role of Film Rupture During Slow Strain-Rate Stress Corrosion Cracking Testing" ASTM STP 665 (1979).
18. Abraham, P. M., T. S. Elleman and K. Verghese, Diffusion and Trapping ofTritium in Grainboundaries of 304L Stainless Steel T. Nud. Mat. 73:77 (1978).
19. Calder R. D, T. S. Elleman and K. Verghese, Grain Boundary Diffusion ofTritium in 304- and 316- Stainless Steels, T. Nud. Mat. 46:46-52 (1973).
20. Murty, K.L., Y.H. Jung, S.T. Mahmood and D.S. Sarma, Fracture Behavior ofA533B Classl Steel: Effects of Dynamic Strain-Aging and Neutron Irradiation,11th International Conference on Structural Mechanics in Reactor Technology(SMiRT-11), Tokyo, Aug., 1991, paper F12/2.
21. Jung, Y.H., P.S. Godavarti, K. Narendrnath and K.L. Murty, A PersonalComputer Based System to Evaluate J-Integral by a Single Specimen UnloadingCompliance Method - Part 1: Methodology, T. Eng. Frac. Mech.. 29, No.l. 1 (1988).
22. Narendrnath, K., H. Margolin, P.S. Godavarti, Y.H. Jung and K.L. Murty, APersonal Computer Based System to Evaluate J-Integral By a Single SpecimenUnloading Compliance Method - Part II: Results on A533B Class I Steel andCorona-5, T. Eng. Frac. Mech., 30, No.3,349-359 (1988).
23. Godavarti, P.S., K. Narendrnath, Y.H. Jung and K.L. Murry, A PersonalComputer Based System to Evaluate ]-Integral by a Single Specimen UnloadingCompliance Method - III : Software, T. Eng. Fract. Mech.36, 341-353 (1990).